bluuebunny/crossref_metadata_2025_split huggingface dataset:
Contact Fatigue Failure of A Bull Gear
Authors: Tanner G. Mark , Harty James R. 
Published: May 2019

Abstract
A bull gear from a coal pulverizer at a utility failed by rolling-contact fatigue as the result of continual overloading of the gear and a nonuniform, case-hardened surface of the gear teeth. The gear consisted of an AISI 4140 Cr-Mo steel gear ring that was shrunk fit and pinned onto a cast iron hub. The wear and pitting pattern in the addendum area of the gear teeth indicated that either the gear or pinion was out of alignment. Beach marks observed on the fractured surface of the gear indicated that fatigue was the cause of the gear failure. Similar gears should be inspected carefully for signs of cracking or misalignment. Ultrasonic testing is recommended for detection of subsurface cracks, while magnetic particle testing will detect surface cracking. Visual inspection can be used to determine the teeth contact pattern.
Failure of Four Cast Steel Gear Segments
Authors: Goodrich George M. 
Published: May 2019

Abstract
Gears in a strip mining dragline failed in service. The material was identified as a low-alloy (NiCrMoV) steel. SEM analysis indicated that the initial fracture and subsequent fractures resulted from impact or a suddenly applied load. Mechanical testing indicated that the gears had low impact strength. Failure was attributed to low toughness caused by the absence of, or improper, heat treatment. Casting defects identified during metallographic examination were determined to be the fracture initiation site, but were considered less significant than the low as-received impact strength of the material. It was recommended that the equipment manufacturer implement an appropriate heat treatment to meet the impact requirements of the application.
Three-Wheel Motorcycle Frame Failures and Redesign
Authors: Knott Thomas A. 
Published: May 2019

Abstract
Bending fatigue caused crack propagation and catastrophic failures at several locations near the welds on the low-carbon steel tubular cargo box frame of police three-wheel motorcycles. ANSYS finite element analysis revealed that bending stresses in some of the frame members were aggravated by poor detail design between vertical and horizontal tubes. Stresses observed in the ANSYS analysis were not sufficient to cause the onset of fatigue. However when compounded by stress concentration factors and in-service dynamic loading, the frame could have been regularly subjected to stresses over the fatigue limit of the material. A strain gage static loading test verified FEM results, and finite element techniques were applied in the design of reinforcing members to renovate the frames. Material properties were determined and welding procedures specified for the reinforcing members. Inspection intervals were devised to avoid future problems.
Failure of Admiralty Brass Condenser Tubes
Authors: Khatak H.S. , Gnanamoorthy J.B. , Rodriguez P. 
Published: May 2019

Abstract
Leaks developed in 22 admiralty brass condenser tubes. The tubes were part of a condenser that was being used to condense steam from a nuclear power plant and had been in operation for less than 2 years. Analysis identified three types of failure modes: stress-corrosion cracking, corrosion under deposit (pitting and crevice), and dezincification. Fractures were transgranular and typical of stress-corrosion cracking. The primary cause of the corrosion deposit was low-flow conditions in those parts of the condenser where failure occurred. Maintenance of proper flow conditions was recommended.
Failure of Three Cyclone Separators
Authors: Goodrich George M. 
Published: May 2019

Abstract
Three 1006 carbon steels team/water separators failed in a boiler in installation after several years of service. Annual inspection had revealed no evidence of deterioration until the last inspection, when they were removed from service. Metallurgical investigation determined that the separators had deteriorated because of erosion corrosion. Further analysis of the boiler operation revealed that operational changes made in the last year of service caused an increase in velocity of the water/steam mixture. It was recommended that the operating parameters for the boiler be reevaluated and prior levels of operation be reinstituted.
Intergranular Stress-Corrosion Cracking Failure in AISI Type 316 Stainless Steel Dished Ends Near Weld Joints
Authors: Bhattacharya D.K. , Jayakumar T. , Raj Baldev 
Published: May 2019

Abstract
Two AISI type 316 stainless steel dished ends failed through the formation of intergranular stress-corrosion cracks (IGSCC) within a few months of service. The dished ends failed in the straight portions near the circumferential welds that joined the ends to the cylindrical portions of the vessel. Both dished ends were manufactured from the same batch and were supplied by the same manufacturer One of the dished ends had been exposed to sodium at 550 deg C (1020 deg F) for 500 h before failure due to sodium leakage was detected. The other dished end was used to fabricate a second vessel that was kept in storage for 1 year Clear evidence of sensitization was found in areas where IGSCC occurred. Sensitization was extensive in the dished end that had been exposed to sodium at high temperature, and it occurred in a narrow band similar to that typical of weld decay in the dished end that had been kept in storage. Solution annealing was recommended to relieve residual stress, thereby reducing the probability of failure. It was also recommended that the carbon content of the steel be lowered, i.e., that a 316L grade be used.
Alkaline-Type Boiler Tube Failures Induced by Phosphate Water Treatment
Authors: Islam Moavinul 
Published: May 2019

Abstract
Tube failures occurred in quick succession in two boiler units from a bank of six boilers in a refinery. The failures were confined to the SAE 192 carbon steel horizontal support tubes of the superheater pack. In both cases, the failure was by perforation adjacent to the welded fin on the crown of the top tubes and located in an area near the upward bend of the tube. The inside of all the tubes were covered with a loosely adherent, black, alkaline, powdery deposit comprised mainly of magnetite. The corroded areas, however, had relatively less deposit. The morphology of the corrosion damage was typical of alkaline corrosion and confirmed that the boiler tubes failed as a result of steam blanketing that concentrated phosphate salts. The severe alkaline conditions developed most probably because of the decomposition of trisodium phosphate, which was used as a water treatment chemical for the boiler feed water.
Caustic-Induced Stress-Corrosion Cracking of a Flue Gas Expansion Joint
Authors: Hahn Sarah Jane 
Published: May 2019

Abstract
A type 430Ti stainless steel flue gas expansion joint cracked because of caustic-induced stress-corrosion cracking. Energy-dispersive X-ray spectroscope analysis of the fracture surface deposits revealed the presence of sodium and potassium—caustics in hydroxide form. Primary fracture surfaces were all similar in appearance, and a primary crack origin could not be identified. A secondary crack brought to fracture in the laboratory showed brittle, cleavage features rather than classic, tensile overload features. This suggested that the material was embrittled.
Failure of Carbon Steel Superheater Tubes
Authors: Ribble Joseph P. 
Published: May 2019

Abstract
Two superheater tubes from a 6.2 MPa (900 psig) boiler failed in service because of creep rupture. One tube was carbon steel and the other was carbon steel welded to ASTM A213 Grade T22 (2.25Cr-1.0Mo) tubing. The failure in the welded tube occurred in the carbon steel section. Portions of the superheater were retubed five years previously with Grade 722 material. The failures indicated that tubes were exposed to long-term overheating conditions. While the carbon steel tube did not experience temperatures above the lower transformation temperature 727 deg C (1340 deg F), the welded tube did experience a temperature peak in excess of 727 deg C (1340 deg F). The long-term overheating conditions could have been the result of excessive heat flux and /or inadequate steam flow. In addition, the entire superheater bank should have been upgraded to Grade 722 material at the time of retubing.
Failure of a Pipe Slip-on Flange
Authors: Chaudhari Mohan D. 
Published: May 2019

Abstract
A cracked 356 mm (14 in.) diam slip-on flange (Ni-Cr-Mo-V steel) was submitted for failure analysis. Reported results and observations indicated that the flange was not an integral forging or a casting, as specified. It had been fabricated by welding and machining a ring insert within a flange with a larger internal diameter. The flange cracked because the welds between the flange and the insert were inadequate to withstand the bolting pressures. A warning was issued to end users of the flanges, which are being inspected nondestructively for conformance to specifications.
Graphitization-Related Failure of a Low-Alloy Steel Superheater Tube
Authors: Kotwica David J. 
Published: May 2019

Abstract
A carbon-molybdenum (ASTM A209 Grade T1) steel superheater tube section in an 8.6 MPa (1250 psig) boiler cracked because of long-term overheating damage that resulted from prolonged exposure to metal temperatures between 482 deg C (900 deg F) and 551 deg C (1025 deg F). The outer diameter of the tube exhibited a crack (fissure) oriented approximately 45 deg to the longitudinal axis and 3.8 cm (1.5 in.) long. The inner diameter surface showed a fissure in the same location and orientation. Microstructure at the failure near the outer diameter surface exhibited evidence of creep cracking and creep void formation at the fissure. A nearly continuous band of graphite nodules was observed on the surface of the fissure. In addition to the graphite band formation, the microstructure near the failure exhibited carbide spheroidization from long-term overheating in all the tube regions examined. It was concluded that preferential nucleations of graphite nodules in a series of bands weakened the steel locally, producing preferred fracture paths. Formation of these graphite bands probably expedited the creep failure of the tube. Future failures may be avoided by using low-alloy steels with chromium additions such as ASTM A213 Grade T11 or T22, which are resistant to graphitization damage.
Stress-Corrosion Cracking of Stainless Steel Superheater Tubing
Authors: Esmacher Mel J. 
Published: May 2019

Abstract
Several 304H stainless steel superheater tubes fractured in stressed areas within hours of a severe caustic upset in the boiler feedwater system. Tests performed on a longitudinal weld joint, which connected two adjacent tubes in the tertiary superheater bank, confirmed caustic-induced stress-corrosion cracking, promoted by the presence of residual welding stresses. Improved maintenance of check valves and routine inspection of critical monitoring systems (conductivity alarms, sodium analyzers, etc.) were recommended to help avoid future occurrences of severe boiler feedwater contamination. Additional recommendations were to eliminate these short longitudinal weld joints by using a bracket assembly joint between the tubes, use a post-weld heat treatment to relieve residual welding stress or select a more stress-corrosion cracking resistant alloy for this particular application.
Stress-Corrosion Cracking of a Swaged Stainless Steel Reheater Pendent Tube
Authors: Studer Anthony C. , Dickens Robert S. 
Published: May 2019

Abstract
A cold-formed Grade TP 304 stainless steel swaged region of a reheater tube in service for about 8000 hours cracked because of sulfur-induced stress-corrosion cracking (SCC). Cracking initiated from the external surface and a high sulfur content was detected in the outer diameter and crack deposits. Comparison of the microstructure and hardness of the swaged region and unswaged Grade TP 304 stainless steel tube metal indicated that the swaged section was not annealed to reduce the effects of cold working. The high hardness created during swaging increased the stainless steel's susceptibility to sulfur-induced SCC. Because SCC requires water to be present, cracking most likely occurred during downtime or startups. To prevent future failures, the boiler should be kept dry during downtime to avoid formation of sulfur acids, and the swaged sections of the tubes should be heat treated after swaging to reduce or eliminate strain hardening of the metal.
Brittle Fracture Explosive Failure of a Pressurized Railroad Tank Car
Authors: Brown Samuel J. 
Published: May 2019

Abstract
A 127 cu m (4,480 cu ft) pressurized railroad tank car burst catastrophically. The railroad tank was approximately 18 m (59 ft) long (from 2:1 elliptical heads), 3 m (10 ft) in OD, and 16 mm (0.63 in.) thick. The chemical and material properties of the tank were to comply with AAR M-128 Grade B. As a result of the explosive failure of the tank car, fragments were ejected from the central region of the car between the support trucks from ground zero to a maximum of approximately 195 m (640 ft). The mode of failure was a brittle fracture originating at a preexisting lamination and crack in the tank wall adjacent to the tank nozzle. The mechanism of failure was overpressurization of the railroad tank car caused by a chemical reaction of the butadiene contents. The interrelationship of the mode, mechanism, and consequences of failure is reviewed to reconstruct the sequence of events that led up to the breach of the railroad tank car. Means to prevent similar reoccurrences are discussed.
Fatigue Failure at Fillet-Welded Nozzle Joints in a Type 316L Stainless Steel Tank
Authors: Bhattacharya D.K. , Ray S.K. , Rodriguez Placid 
Published: May 2019

Abstract
Upon arrival at the erection site, an AISI type 316L stainless steel tank intended for storage of fast breeder test reactor coolant (liquid sodium) exhibited cracks on its shell at two of four shell/nozzle fillet-welded joint regions. The tank had been transported from the manufacturer to the erection site by road, a distance of about 800 km (500 mi). During transport, the nozzles were kept at an angle of 45 deg to the vertical because of low clearance heights in road tunnels. The two damaged joints were unsupported at their ends inside the vessel, unlike the two uncracked nozzles. Surface examination showed ratchet marks at the edges of the fracture surface, indicating that loading was of the rotating bending type. Electron fractography using the two-stage replica method revealed striation marks characteristic of fatigue fracture. The striations indicated that the cracks had advanced on many “mini-fronts,” also indicative of nonuniform loading such as rotating bending. It was recommended that a support be added at the inside end of the nozzles to rigidly connect with the shell. In addition to avoiding transport problems, this design modification would reduce fatigue loading that occurs in service due to vibration of the nozzles during filling and draining of the tank.
Failure of a Martensitic Stainless Steel Ball Valve
Authors: Kaul Rakesh , Muralidharan N.G. , Kasiviswanathan K.V. , Raj Baldev 
Published: May 2019

Abstract
Repeated failures of high-pressure ball valves were reported in a chemical plant. The ball valves were made of AFNOR Z30C13 martensitic stainless steel. Initial examination of the valves showed that failure occurred in a weld at the ball/stem junction end of austenitic stainless steel sleeves that had been welded to the valve stem at both ends. Metallographic examination showed that a crack had been introduced into the weld by improper weld heat treatment. Stress concentration at the weld location resulting from an abrupt change in cross section facilitated easy propagation of the crack during operation. Proper weld heat treatment was recommended, along with avoidance of abrupt change in cross section near the weld. Due penetrant testing at the ball stem junction before and after heat treatment was also suggested.
Cracking in a Steam Turbine Rotor Disk
Authors: Colwell Richard L. 
Published: May 2019

Abstract
An A-470 steel rotor disk was removed from the high-pressure portion of a steam turbine-powered compressor after nondestructive testing revealed cracks in the shoulder of the disk during a scheduled outage. Samples containing cracks were examined using various methods. Multiple cracks, primarily intergranular were found on the inlet and outlet faces along prior-austenite grain boundaries. The cracks initiated at the surface and propagated inward. Multiple crack branching was observed. Many of the cracks were filled with iron oxide. X-ray photoelectron spectroscopy indicated the presence of sodium on crack surfaces, which is indicative of NaOH-induced stress-corrosion cracking. Failure was attributed to superheater problems that resulted in caustic carryover from the boiler. Two options for disk repair, installing a shrink-fit disk or applying weld buildup, were recommended. Weld repair was chosen, and the rotor was returned to service; it has performed for more than 1 year without further incident.
Failure Analysis of a Cracked Low-Pressure Turbine Blade
Authors: Ciulik J. 
Published: May 2019

Abstract
A cracked, martensitic stainless steel, low-pressure turbine blade from a 623 MW turbine generator was found to exhibit fatigue cracks during a routine turbine inspection. The blade was cracked at the first notch of the fir tree and the cracks initiated at pits induced by chloride attack. Examination of the blade microstructure at the fracture origins revealed oxide-filled pits and transgranular cracks. The oxide filled cracks appeared to have originated at small surface pits and probably propagated in a fatigue or corrosion-fatigue fracture mode. It was recommended that the sources of the chlorides be eliminated and that the remaining blades be inspected at regular maintenance intervals for evidence of cracking.
Failure of Non-Magnetic Retaining Ring in a High-Speed Generator Rotor
Authors: Sherlock Thomas P. , Jirinec Michael J. 
Published: May 2019

Abstract
A shrunk-fit 18 Mn-5Cr steel retaining ring failed without warning during normal unit operation of a 380 MW electrical generator. The cause of the ring failure was determined to be intergranular stress-corrosion cracking (IGSCC) because of the high strength of the ring material and the presence of moist hydrogen used to cool the ring. Factors which promoted the failure were higher than normal strength levels in the ring material, lower than normal ring operating temperatures, possible moisture in the lubrication oil system, periodic poor performance of the hydrogen dryers, and a ring design which allowed water to become trapped in a relief groove. These factors caused pitting in the ring in an estimated 100 hours of operation. The ring had been inspected previously 18 months prior to the failure and no defects or pitting were found. Calculations showed that a 0.127-cm (0.050-in.) deep pit could grow to a critical size in 3000 to 4000 hours of operation. To prevent further failures, it was recommended that the ring be replaced with an 18 Mn-18Cr alloy with superior resistance to IGSCC. A program of periodic inspection and replacement of other retaining rings in the system was also recommended.
Fatigue Cracking of Gas Turbine Diaphragms
Authors: Fleck N.A. 
Published: May 2019

Abstract
Several compressor diaphragms from five gas turbines cracked after a short time in service. The vanes were constructed of type 403 stainless steel, and welding was performed using type 309L austenitic stainless steel filler metal. The fractures originated in the weld heat-affected zones of inner and outer shrouds. A complete metallurgical analysis was conducted to determine the cause of failure. It was concluded that the diaphragms had failed by fatigue. Analysis suggests that the welds contained high residual stresses and had not been properly stress relieved. Improper welding techniques may have also contributed to the failures. Use of proper welding techniques, including appropriate prewelding and postwelding heat treatments, was recommended.
Fatigue Fracture of a Precipitation-Hardened Stainless Steel Actuator Rod End
Authors: Levy Eli 
Published: May 2019

Abstract
A 17-4 PH steering actuator rod end body broke during normal take-off. Results of failure analysis revealed that the wall thickness of the race was much below the design limits, thus causing the race to rest on the body's swaged edges rather than on the load carrying centerline of the body. This assembly condition generated abnormal high loads on the swaged edges, ultimately resulting in fatigue failure. To prevent a recurrence of similar failure in the future, the dimensions of the race in the spherical bearing were changed, no further failure occurred.
Metallurgical Analysis of Steam Turbine Rotor Disc
Authors: Hodas Leonard J. 
Published: May 2019

Abstract
Numerous cracks observed on the surface of a forged A470 Class 4 alloy steel steam turbine rotor disc from an air compressor in a nitric acid plant were found to be the result of caustic induced stress-corrosion cracking (SCC). No material defects or anomalies were observed in the disc sample that could have contributed to crack initiation or propagation or secondary crack propagation. Chlorides detected in the fracture surface deposits were likely the primary cause for the pitting observed on the disc surfaces and within the turbine blade attachment area. It was recommended that the potential for water carryover or feedwater induction into the turbine be addressed via an engineering evaluation of the plant's water treatment procedures, steam separation equipment, and start-up procedures.
Failure of a Crane Long-Travel Worm Drive Shaft
Authors: Wellington K.G. 
Published: May 2019

Abstract
A crane long-travel worm drive shaft was found to be chipped during unpacking after delivery. Chemical analysis showed that the steel (EN36A with a case depth of 1 mm, or 0.04 inch did not meet specifications. Magnetic particle inspection revealed a crack on the side of the shaft opposite the chip. Metallographic examination indicated that the case depth was approximately 2 mm (0.08 in.) and that a repair weld of an earlier chip had been made in the cracked area. The chipping was attributed to excessive case depth and rough handling. It was recommended that the shaft be returned to the manufacturer and a replacement requested.
Fatigue Failure of a Circulating Water Pump Shaft
Authors: Hare Joyce M. 
Published: May 2019

Abstract
A type 410 stainless steel circulating water pump shaft used in a fossil power steam generation plant failed after more than 7 years of service. Visual examination showed the fracture surface to be coated with a thick, spalling, rust-colored scale, along with evidence of pitting. Samples for SEM fractography, EDS analysis, and metallography were taken at the crack initiation site. Hardness testing produced a value of approximately 27 HRC. The examinations clearly established that the shaft failed by fatigue. The fatigue crack originated at a localized region on the outside surface where pitting and intergranular cracking had occurred. The localized nature of the initial damage indicated that a corrosive medium had concentrated on the surface, probably due to a leaky seal. Reduction of hardness to 22 HRC or lower and inspection of seals were recommended to prevent future failures.